Phase separation in polymer solutions. I. Liquid-liquid phase
separation of PPO poly (2, 6-dimethyl 1, 4-phenylene oxide) in
binary mixtures with toluene and ternary mixtures with toluene and
ethyl alcoholJ. POLYMER SCI.: PART C NO. 38,73-86 (1972)
PHASE SEPARATION IN POLYMER SOLUTIONS. I. LIQUID-LIQUID PHASE
SEPARATION OF PPO POLY (2,6-DIMETHYL 1,4-PHENYLENE OXIDE) IN BINARY
MIXTURES WITH TOLUENE AND TERNARY MIXTURES WITH TOLUENE AND ETHYL
P. T. VAN EMMERIK and C. A. SMOLDERS
Twente University of Technology, Enschede, Netherlands
In the system p0ly(2,6-dimethyl-lf 4-phenylene oxide) (PP0)-toluene
three phase sepa- ration lines can be detected: the melting point
cWe. the cloud point curve, and the spinodial. Because
crystallization of PPO occurs very slowly, a phase transition will
always be initiated by liquid-liquid phase separation. Depending
upon the experimental circum- stances two mechanisms are possible,
either nucleation and growth (extremely slowly in this system) or
the spinodial decomposition mechanism. In the system
PPO-tolueneethanol, liquid-liquid phase separation occurs leading
to two bulk liquid fractions. Only in mixtures containing very smal
l concentrations of alcohol can threephase separation c w e s be
detected from which the position of the cloud point curve of the
system PPO-toluene can be confirmed.
Depending upon the experimental circumstances liquid-liquid phase
separa- tion can be initiated by one of the following mechanisms:
nucleation and growth [l], well known in a number of polymer
solvent systems, or spinodial decomposition, which occurs in
certain metal alloys and glasses and is described by the theory of
Cahn . In a few recent articles the onset of the phase
separation of poly (2,6-dimethyl- 1,4phenylene oxide)
(PP0)-caprolactam mix- tures was described and explained by a
spinodial decomposition mechanism [3,4]. An adaption of the theory
of Cahn to solutions of high polymers has been given [ 51 .
The present study was initiated to learn more about the
thermodynamics of liquid-liquid phase separation of PPO-solvent
mixtures. Some results con- cerning the phase equilibria of
PPO-toluene mixtures and PPO-toluene-ethyl alcohol mixtures are
74 EMMERIK AND SMOLDERS
FIG. 1. Liquid ternary system: P, , polymer with chain length n;
P,, polymer with chain length m (m * n); OP,, complete miscibility;
OP,, limited miscibility; KLM, cloud point cuIVe.
The free enthalpy (Gibbs free energy) of mixing AG, of any closed
system in stable equilibrium at constant pressure and temperature
can be represented graphically for binary and ternary systems. In
regions where AG, of the homogeneous solutions is higher than that
of a combination of two phases the minimum free enthalpy of the
system will be given by the phase separated system; the composition
of the phases being given by the tangent phase of the AG, surface.
When all sets of tangent points are projected on the base triangle,
they represent the binodial which is the limit of stability of the
Another set of characteristic points of the ACm surface are the
inflection points which form the boundary of the concave part of
the free energy surface. Its projection on the base triangle is
called the spinodial. Phase diagrams of this type are
characteristic for a nonsolvent (l)/solvent (2)/solute (3) system
and have been extensively discussed by Tompa [ 6 ] .
It is clear that the composition diagram will have three regions:
1) A region where all solutions are stable (AC, concave upwards).
the area outside the binodial. 2) A metastable region (AGm is still
concave upwards, but fluctuations of a
certain composition and size, may initiate phase separation). This
is the area between the binodial and the spinodial.
PHASE SEPARATION 15
3) An unstable region (AG, is concave downwards). This is the area
within the spinodial, where spontaneous phase separation always
takes place by the spinodial mechanism.
A polymer solution actually represents a multicomponent system and
a graphical representation of AG, would require more than three
dimensions. Several authors [7,8] have shown that a
three-dimensional diagram for a liquid ternary system brings out
most of the essential features of the behavior of polydisperse
polymer solutions. A phase diagram for a polymer solution is shown
in Figure 1. At the temperatures considered, OP1 and 0P2 show
complete and limited miscibility, respectively. OX represents all
systems containing a certain mixture of PI and P2, which is the
actual polymer sample, and the solvent. The plane TOX intersects
the binodial surface; the resulting curve is called the cloud point
curve. The spinodial must be situated below the cloud point curve,
touching the cloud point curve in the critical point.
For most polymer solvent systems the critical point and the maximum
of the cloud point curve are situated between 2 and 15% by weight
polymer. Liquid-liquid phase separation seems to occur in most
cases by nucleation and growth which is followed by coalescence of
the separated liquid phase to give two bulk liquid layers in the
end. If nucleation and growth is a very slow process it is possible
to cool a solution below the spinodial without extensive nucleation
taking place. In that case liquid-liquid phase separation will be
initiated by the spinodial mechanism.
The materials used were: PPO: M, = 25,000, M, = 39,000, Tg = 220°C;
to1uene;lethyl alcohol PA.
Homogeneous mixtures of PPO-toluene and/or ethyl alcohol were made
by weighing the appropriate amounts in small Pyrex glass tubes
which were degassed, flushed with nitrogen, degassed again and
sealed under vacuum at liquid nitrogen temperature. The sealed
glass tubes were heated in an oil bath at 150°C for a minimum 24 hr
in order to get homogeneous liquid mixtures. Phase separation
points were determined visually by cooling the thermostated bath by
1°C every 10 min or by 1°C every 48 hr. After phase separation set
in, the mixtures were kept at a temperature well below the phase
separation temperature for at least 24 hr before the phase
separation points were determined anew by heating the demixed
solutions at the rate of 1°C every 10 min or of 1' every 48 hr.
Equilibrium concentrations could be determinedfor the dilute phase
only. Solutions were kept at the appropriate demixing temperature
for at least 2 weeks. By centrifugation at that temperature the
dilute and the concentrated phase were separated. The percentage of
PPO in the dilute phase could easily be determined by evaporation
of the toluene. The concentrated phase could never be made
completely free of the dilute phase even after prolonged periods of
centrifugation, hence determination of the former phase's
concentration was not feasible.
76 EMMERIK AND SMOLDERS
When a homogeneous mixture of PPO in toluene is cooled two
transition temperatures will be found depending upon the cooling
rate. The phase separation temperatures for different mixtures
observed during cooling at 1°C per 10 min are shown in Figure 2 as
curve A, which is characterized by the experimental phenomenon of
instantaneous complete demixing with- out formation of nuclei being
detectable under the light microscope.
The transition temperatures observed during extremely slow cooling
at 1°C each 48 hr are shown as curve B in Figure 2. When phase
separation has set in and the solution is heated again after 24 hI
of waiting, a third curve of transition temperatures will be found,
curve C in Figure 2. This latter curve is found independently of
the rate of heating.
A different way to determine curve A is quenching a homogeneous
mixture of PPO-toluene to a low temperature and to determine the
time which elapses before phase separation becomes visible. At
higher final temperatures this incipient precipitation time
suddenly increases to high values as shown in Figure 3.
A 5 min time limit has been adopted for the estimation of the
temperatures shown in curve A in Figure 2. The curves A and B are
both cut off by the glass transition temperature line. Homogeneous
solutions cooled to appropriate
0 10 20 30 40 50 60 - weight percentage of polymer
FIG. 2. Phase separation curves of PPatoluene solutions: (X) phase
separation tempera tures observed during cooling at 1°C per 10 min;
(0) phase separation temperatures observed during cooling at 1°C
per 48 hr; (0) melting point curve; (- -) glass transition
PHASE SEPARATION 77
0 10 20 - T ( ' c )
FIG. 3. Incipient precipitation time as a function of the quenching
temperature of a 20% of weight PPO-toluene solution.
temperatures between curve B and C will remain homogeneous even
after prolonged periods of at least 4 months.
Cooled at temperatures between B and A liquid-liquid phase
separation occurs by way of nucleation and growth (Fig. 4),
nucleation occurring after induction times which approach infinity
at temperatures near curve B and which fall to zero when the
temperature approaches curve A .
The phase equilibrium curves of different PPO-toluene mixtures have
been determined. Due to experimental difficulties the percentage of
weight PPO could be determined in the dilute phase only (Fig. 5) .
These equilibrium curves finish in curve B of Figure 2,
The phase separation curves for different mixtures of
PPO-tolueneethyl alcohol are shown in Figures 6 , 7 , 8 , and 9. In
Figure 6 in each solution
weight percent PPO
weight percent ethyl alcohol = 1
If the total amount of PPO t ethyl alcohol exceeds 40% of the total
weight, liquid-liquid phase separation only occurs, independent of
the cooling rate. The final situation was always characterized by
two bulk liquid fractions, a
78 EMMERIK AND SMOLDERS
FIG. 4. Liquid-liquid phase separation by nucleation and growth of
a 30% of weight PPO-toluene solution at T = 48°C.
concentrated and a dilute one. If the solutions contained less than
40% of weight PPO + ethyl alcohol, three curves could be observed
in the same way as with PPO-toluene mixtures.
In Figure 7
weight percent toluene
PHASE SEPARATION 79
10 20 30 - weight percentage of polymer
FIG. 5. Phase equilibrium of the dilute phase of demixed 20% of
weight PPOtoluene solution: (0) equilibrium concentration of dilute
phase; (0) phase separation points observed during cooling at 1°C
each 48 hr; ( X ) phase separation points observed during cooling
at 1°C per 10 min.
Only liquid-liquid phase separation was observed leading to two
bulk liquid fractions, phase separation points being independent of
the speed of cooling or heating.
In Figure 8
weight percent toluene
weight percent toluene = 50% constant
Both figures show the same features as Figure 6 . In regions where
the concentration of ethyl alcohol is low three curves could be
determined. In the other regions liquid-liquid phase separation
DISCUSSION OF RESULTS
In the literature many polymer-liquid systems have been discussed.
In all those systems it was quite clear whether the phase
separation curve was a melting point curve or a liquid-liquid phase
separation curve. PPO belongs to the
80 EMMERIK AND SMOLDERS
60 40 0 - weight percentage of polymer weight percentage
FIG. 6. Phase separation curves of PPO-tolueneethanol solutions:
(v) cloud point curve; (@)
melting point curve; (A) spinodial.
class of slowly crystallizing polymers [lo]. It cannot be
crystallized by thermal treatment but may show crystallization when
brought into contact with certain organic liquids [ 1 I] . Even
then crystallization occurs very slowly.
When the system €TO-toluene is considered, the problem is how to
interpretate the curves A, B, and C.
We believe that curve B represents the cloud point curve for the
1) ' h e end of the different liquid-liquid phase separation curves
of the system €TO-tolueneethyl alcohol in the PPO-toluene plane is
always situated on curve B.
2) When homogeneous mixtures of PPO-toluene are cooled to the appre
priate temperature between cunes A and B phase separation occurs
PHASE SEPARATION 81
20 4b 6b 8'0 &I - weight percentage of polymer
FIG. 7. Cloud point curve of PPOtoluene-ethanol solutions. In each
solution the wt % ethanol = %toluene.
nucleation and growth. The spherical areas of the concentrated
phase (Fig. 4) do not show any properties of spherulites (they do
not show the Maltese cross under polarized light, e.0.). Only after
prolonged waiting does it lighten up a bit, indicating that
crystallization of the concentrated areas eventually takes place
after liquid-liquid phase separation has begun.
3) The phase equilibrium curve of the dilute phase ends in curve B
(Fig. 5 ) which is characteristic for liquid-liquid phase
82 EMMERIK AND SMOLDERS
60 40 20 0 - 80 weight percentage of polymer+ toluene
FIG. 8. Phase separation curves of PPO-tolueneethanol solutions. In
wt %toluene - 7 wt%PPO 3
_ - (A) cloud point curve; (0) melting point curve; (v)
4) Homogeneous solutions cooled rapidly at temperatures below curve
A demix instantaneously but will become homogeneous again at
temperatures corresponding to curve B when heated immediately after
completion of phase separation.
Curve A represents the spinodal because 1) in homogeneous solutions
of PPO in toluene rapidly cooled to tempera-
tures on or below curve A nucleation has never been detected but
structures well known for spinodial decomposition have been
2) homogeneous mixtures of PPO in toluene demix instantaneously
when cooled to any temperature below curve A (except when the
quenching temperature is below the Tg of the mixture).
PHASE SEPARATION 83
the wt %
Curve C represents the melting point curve since 1) the
concentrated areas formed during nucleation and growth lighten up
bit under polarized light when kept at the demixing temperature,
indicating that crystallization is gradually taking place;
2) if these concentrated areas are kept at the demixing temperature
for at least 24 hr the concentrated phase can be separated from the
dilute phase. After careful drying the residue which is pure €TO,
does show some crystallinity;
3) if demixed solutions are kept at the demixing temperature for
various times, the transition temperatures determined when the
solutions are heated again, are always situated on curve C, never
at temperatures between B and C.
The most remarkable feature of the system PPO-toluene is the cloud
point curve B in Figure 2, which does not show a maximum up to 75%
of weight PPO, which is quite different from cloud point curves
known from literature. A possible explanation for this phenomenon
is an unusual dependence of the interaction between polymer
segments and solvent molecules on concentration and temperature
. Taking curves A and B into account, we propose that Figure 10
depicts the phase diagram of the liquid system PPO-toluene.
The phase separation curves of the system PPO-toluene-ethyl alcohol
represent the cloud point curves of this system. Only in regions
close to the PPO-toluene plane splitting up into three curves takes
place. Curve C is again the melting point curve, curve B is the
cloud point, and curve A is the spinodial.
Cross sections of the diagram of this system at different
temperatures are given in Figure 11. From Figure 11 it can be read
that depending upon the
FIG. 10. Ternary liquid diagram for PPO-toluene: P, , polymer chain
length n; P, , polymer chain length m (m * n); S, sokent; PQ, cloud
point curve; RS, spinodial curve.
T = 140
FIG. 11. Cross sections at different temperatures of the phase
diagram of the system PPO-tolueneethanol.
PHASE SEPARATION 85
temperature a considerable amount of the extremely poor solvent
ethyl alcohol can be added to mixtures of PPO-toluene without
causing a phase separation. If phase separation occurs the final
situation is characterized by two bulk liquid fractions except for
regions close to the PPO-toluene plane. Nucleation and growth are
not retarded any more and the spinodial cannot be measured.
Even small amounts of ethyl alcohol causes a considerable
depression of the melting points until below the liquid-liquid
separation line. Only in solutions containing small amounts of
ethyl alcohol compared to toluene, is it possible to determine
experimentally the three curves mentioned above.
For temperatures above 130°C the phase diagram in Figure 11 is the
same as discussed by Tompa  for the general case
polymer/solvent/nonsolvent. Below 130°C the diagram differs from
this system and is also different when compared with the diagram of
the general system polymer/nonsolvent/nonsolvent as discussed by
Tompa and Scott [ 121 .
From these results it can be inferred that in the system
PPO-toluene the amorphous separation range is situated close to the
melting point curve of the crystalline polymer. In their paper on
classification of polymer solvent systems Papkov and Yefimova [ 141
give a general description of such a system that is in good
accordance with the system PPO-toluene. If a homogeneous solution
of such a system is cooled to a temperature below its melting point
phase separation will not occur because the rigid chains of the
polymer prevent the precise molecular packing necessary for
crystallization. Upon further cooling the metastable range with
respect to liquid-liquid phase separation is entered into where a
simple piling up of molecules is sufficient to reach the required
critical concentration and size. As a result liquid-liquid phase
separation is initiated by nucleation and growth and two amorphous
phases are formed. One phase (the most concentrated one)
corresponds now to very high supersaturation with respect to
crystallization and creates conditions for spontaneous nucleation
of the crystalline phase.
The spinodial can only be detected if during cooling nucleation
occurs extremely slowly. In PPO-toluene solutions this is actually
the case and spinodial decomposition patterns are observed. A gel
is formed which is builtup of interconnected areas of the
concentrated and the dilute phase. The concentrated areas
correspond again to high supersaturation with respect to
crystallization and crystallizes. As a result the gel changes into
a rigid mass, in this way preserving the spinodial pattern. Further
microscopic and light scattering experiments are in good agreement
with the experiments and conclusions described in this article
[ l ] M. Volmer and A. Weber, Z. Phys. &ern., 119,277 (1925). [
2 ] J. W. Cahn, lkzns. Met. Soc. AIME, 242,166 (1968).
86 EMMERIK AND SMOLDERS
[ 31 J. J. van Aartsen and C. A. Smolders, Europ. Polym. J. 6, 1105
(1970).  C. A. Smolders, J. J. van Aartsen, and A. Steenbergen,
Kolloid-Z. Z. Polym., 243, 14
(1971).  J. J. van Aartsen, Europ. Polym J., 6,919 (1970). 
H. Tompa, Polymer Solutions, Buttworths, London, 1956. [ 71 R
Koninweld, Advun. a l l . Interface Sci, 2, 15 1 (1 968).  G.
Rehage, D. Mollex, and 0. Emst, Mikromol. Chem, 88, 232 (1965). [
91 P. T. van Emmerik and C. A. Smolders, to be published. [lo] J.
Boon and E. P. Magrd, ZUPACZnter. Symp., vol. ZZ, Leiden, 834
(1970). [ 111 F. E. Karasz and J. M. O'Reilly, J. Polym. Sci, 83,
561 (1956).  R. L. Scott, J. Chem Phys., 17, 3,268 (1949). [
131 P. T. van Emmerik and C. A. Smolders, J. Polym Sci., C, 39, to
be published.  S. P. Papkov and S. G. Yefimova, Fuserforsch
Textil. tech. Sow: Beitrage, 4, 118